Graphite nanoplatelet chemical cross-linking by elemental sulfur
© Carotenuto et al.; licensee Springer. 2013
Received: 31 December 2012
Accepted: 5 February 2013
Published: 20 February 2013
Graphite nanoplatelets (GNPs) react with elemental sulfur to provide a mechanically stable, spongy material characterized by good electrical conductivity and high surface development; such unique property combination makes these novel nanostructured materials very useful for applications in different technological fields. The carbon-sulfur reaction can be accurately investigated by thermal analysis (differential scanning calorimetry and thermogravimetric analysis) and energy-dispersive X-ray spectroscopy combined with scanning electron microscopy. The thermal treatment required for the formation of electrically conductive monosulfur connections among the GNP unities has been investigated.
81.05.Ue, 81.05.Rm, 81.16.Be
KeywordsGraphite nanoplatelets Sulfur Mechanical stabilization Calorimetry
Graphene, a single layer of carbon atoms arranged in a hexagonal network, is a 2D nanostructure with outstanding physical properties . The successful isolation of graphene has had great interest for experimental investigations and has opened the way to a wide range of novel technological applications . Recent studies have been directed toward using graphite nanoplatelets (GNPs) and graphene as a substrate to support nanostructures (e.g., quantum dots, metal catalysts, magnetic nanoparticles, etc.) because of their wide surface area, chemical stability, mechanical strength, and flexibility [2–4].
sp2 carbon nanoforms (e.g., fullerenes, CNTs, graphite nanoplatelets, and graphene) can be chemically cross-linked and polymerized by reaction with elemental sulfur. The resulting synthetic solid phases can be considered as a sort of three-dimensional polymers of sulfur and structurally complex carbon-based monomers. This carbon-sulfur chemical reaction may result in a certain importance in the preparation of novel bulky nanostructured materials . For example, a highly spongy graphite-based material (graphite aerogels) can be prepared by drying concentrated GNP colloids, achieved by exfoliation of expanded graphite in nonpolar liquids with ultrasounds . This novel material is quite fragile and has a measured apparent density of 0.5 g/cm3. A mechanical stabilization treatment is required to exploit this system in technological applications. The carbon-sulfur chemical reaction can be advantageously used for the mechanical stabilization of the very fragile spongy graphite material. The introduction of sulfur in this spongy graphite structure is quite simple since the sulfur molecules (S8) are soluble in nonpolar organic media (hydrocarbons, etc.), and it can be dissolved in the GNP colloid before the drying process. Then, the dry GNP-based material is heated at ca. 180°C to allow the sulfur molecules to open, producing sulfur bi-radicals (∙ S8∙) which bridge the graphene layers of closed nanoplatelets . In particular, the ring of sulfur molecule (S8) breaks at a temperature of ca. 169°C, producing linear sulfur bi-radical fragments, and such endothermal process is named as λ-transition . The permanence of the system at temperatures above the λ-transition allows the polysulfur molecular chains (C-(S) n -C) to break successively and the generated sulfur radicals to react again with the edges of graphene sheets above to achieve a high density of monosulfur chemical cross-links (C-S-C) between them. The monosulfur bridges allow electron delocalization among the graphene sheets, and therefore, they represent a sort of electrical connections in the material. When the spongy graphite is devoted to technological applications in the electrical/electronic field (e.g., supercapacitor electrodes, battery cathodes, electrodes for electrolytic cells, etc.) , the presence of monosulfur bridges among the GNP unities is a very convenient characteristic. In addition, the material stiffness is related to the length of sulfur bridges, and monosulfur connections lead to a much more rigid and tough material.
Expandable graphite flakes (Asbury, Asbury, NJ, USA) underwent a thermal shock at 750°C for 3 min in a muffle furnace to produce expanded graphite (worm-like graphite). As-received elemental sulfur (99.9%, Sigma-Aldrich, Milan, Italy) was dissolved in octane (purum, Carlo Erba Reagents, Milan, Italy), and the expanded graphite filaments were added step by step to this sulfur solution during an ultrasound processing of the liquid system, done with a horn sonicator (20 KHz, 200 W, model UW2200, Bandelin Sonoplus, Berlin, Germany) at room temperature. The resulted expanded graphite filaments were completely converted to GNPs after ultrasound application. The final product was a sort of paste, which was dried in air at room temperature to produce a highly porous graphite/sulfur mixture, successively annealed in oven at 300°C in order to cross-link the material.
Dynamic calorimetric tests were carried out by a differential scanning calorimeter (DSC; Q2920, TA Instruments, New Castle, DE, USA). Measurements were performed under fluxing nitrogen at a rate of 10°C/min ranging from 20°C to 300°C.
Thermogravimetric analysis (TGA) was carried out using a thermobalance (Q5000, TA Instruments). In particular, the samples were heated from 30°C to 800°C at a rate of 10°C/min in fluxing air.
Results and discussion
Thermodynamic properties of the S/GNP system obtained by DSC
T α → β
ΔHα → β
The isothermal annealing of the reactive sulfur/GNP system at temperatures higher than 160°C allows a more or less complete conversion of polysulfur bridges (C-S8-C) to monosulfur bridges (C-S-C) which are sort of electrical connections between the graphene planes because conjugation is possible through the sulfur atom. When the GNP-based aerogels are devoted to electrical applications (e.g., electrodes for batteries and supercapacitors, electrolysis cells, etc.), such type of chemical cross-linking results are extremely convenient.
The λ-transition is characterized by a clearly visible endothermic signal (the enthalpy change is 1.10 J/g), and it can be detected also in the DSC analysis of S/GNP mixtures (see Figure 3 (thermograms a and b)). Consequently, important information on the chemical interaction between sulfur and GNP can be obtained by DSC analysis.
The first reaction step involves the cleavage of the S-S bond with the formation of two sulfur radicals. This elemental reaction is reversible and has a slow specific rate. In the second elemental reaction, one of the two sulfur radicals is added to the carbon-carbon double bond with the formation of S-C bond and one carbon radical. Such reaction should have a fast rate because an unstable reactant (the sulfur radical) is involved. In the last elemental reaction, the carbon radical combines with the second sulfur radical with the formation of a new S-C bond. Also, this step should be very fast because the combination of two radicals is involved. The full reaction rate depends only on the slowest step which is characterized by a first-order kinetic; consequently, the rate expression is −d[S-S]/dt = k[S-S], which after integration provides an exponential recovery law (α = 1 − e−kt). Finally, according to the DSC analysis, the S/GNP chemical interaction is of the first kinetic order, and the involved mechanism is a direct reaction between the sulfur radicals generated at λ-transition and the sp2 carbon atoms located at the edges of the graphite nanocrystals.
In conclusion, the graphite nanoplatelets are very useful nanostructured materials that can be easily prepared by the oxidation-expansion-exfoliation process. GNP-based aerogels can be simply obtained by drying the concentrated GNP colloidal suspensions, and the introduction of elemental sulfur in the GNP aerogel followed by an adequate thermal annealing treatment allows a very good mechanical stabilization of the material by formation of monosulfur and polysulfur bridges between adjacent GNP unities.
GC is a senior researcher of the Italian National Research Council, Institute for Composite and Biomedical Materials. His present research interests are in the field of advanced functional materials based on polymer-embedded inorganic nanostructures. In particular, his activity concerns the development of new chemical routes for the controlled synthesis of metal and semiconductor clusters in polymeric matrices, the fabrication of devices based on properties of nanoscopic objects (e.g., luminescence of quantum dots, tunable surface plasmon absorption of nano-sized noble metal alloys, etc.), and the investigation of mechanisms involved in atomic and molecular cluster formation in polymeric media (nucleation, growth, aggregation, etc.) by optical and luminescence spectroscopy. He has authored 150 research articles published in international journals, ten patents, and many conference papers. He is the editor of two Wiley books devoted to metal-polymer nanocomposites and is a member of the editorial board of different scientific journals.
VR received her PhD in chemical engineering at the University of Salerno-Italy. During her PhD study, she spent a research period at the Institute of Polymer and Fibers in Moldal (Goteborg-Sweden), where she studied the effect of nanoparticle addition on the nanofibers obtained with electrospinning technique. She was a consulting engineer at the Department of Chemical and Food Engineering - University of Salerno for the project ‘Innovative technologies for production of new nanocomposite and carbon nanotubes.’ Currently, she is a scientific consultant of the Italian National Research Council, Institute for Composite and Biomedical Materials, for the project ‘AUTOSUPERCAP’ (Development of high energy/high power density supercapacitors for automotive applications). Her research interests include the preparation of nanostructure carbon materials.
SDN received his BS degree in physics from the University of Naples “Federico II”, Italy, in 1982. From 1983 to 1987, he was a system analyst at Elettronica (Rome) and Alenia (Naples). Since 1988, he has been a senior researcher of the Institute of Cybernetics “E. Caianiello” of the National Council of Research (CNR). Since 2010, he has been a member of the optical staff of the Italian National Institute of Optics (INO-CNR). He has been a scientific coordinator of the research project ‘Imaging Techniques for Studying and Analyzing Microstructured Materials’ of the CNR Department of Material and Devices. He has been a coordinator of the research unit based at the Institute of Cybernetics in the framework of the Italian National Research FIRB programme: Photonic Microdevices in Lithium Niobate. He has contributed to about 300 technical papers in peer-reviewed international journals, book chapters, and conference proceedings. He has served in program committees of several international conferences and has been a referee for various journals in the field of optics and theoretical physics. His research interests include the development and applications of non-destructive methods for material evaluation, optical metrology, theoretical modeling of laser beam propagation in heterogeneous media and nanostructured composites, nonlinear optical effects in cavity, quantum optics, laser-plasma interactions, spectroscopic techniques for nanostructured material, and development of quantum-like models in mesoscopic physics.
LN is President of the National Research Council of Italy, professor emeritus at the University of Naples “Federico II”, and adjunct professor at the Universities of Connecticut in Storrs and Washington in Seattle. He has a prepost of the Schools of Science, Engineering, and Architecture of the University of Naples “Federico II”. He is the author of more than 500 papers in scientific journals and 35 patents and is also the editor of 15 books. He is a member of the editorial boards of many scientific journals. He was awarded the SAMPE (Society for the Advancement of Materials Technology) honor certificate, the ‘G. Dorsi’ and ‘Scanno’ prizes, and the gold medal of the Academy of the Forty. LN significantly contributed to the development of knowledge in the field of composite materials, rheology, energy and mass diffusion through polymers, and materials for biomedical application.
We acknowledge Sherlyn C. Machica for her careful reading of the manuscript.
- Geim AK, Novoselov KN: The rise of graphene. Nat Mater 2007, 6: 183–191. 10.1038/nmat1849View Article
- Wang H, Casalongue S: Ni(OH)2 nanoplates grown on graphene as advanced electrochemical pseudocapacitor materials. J Am Chem Soc 2010, 132: 7472–7477. 10.1021/ja102267jView Article
- Carotenuto G, De Nicola S: Mechanical properties of low-density polyethylene filled by graphite nanoplatelets. Nanotechnology 2012, 23: 1–8.View Article
- Wang X, Tabakman SM: Atomic layer deposition of metal oxides on pristine and functionalized graphene. J Am Chem Soc 2008, 130: 8152–8153. 10.1021/ja8023059View Article
- Ji X, Lee KT, Nazar LF: A highly ordered nanostructured carbon–sulphur cathode for lithium–sulphur batteries. Nat Mater 2009, 8: 500–506. 10.1038/nmat2460View Article
- Xusheng D, Zhong-Zhen Y: New method to prepare graphite nanocomposites. Chem Mater 2008, 20: 2066–2068. 10.1021/cm703285sView Article
- Eichinger BE, Wimmer E: The structure of amorphous sulfur. Macromol. Symp 2001, 171: 45–56. 10.1002/1521-3900(200106)171:1<45::AID-MASY45>3.0.CO;2-NView Article
- Klement W: Study of the λ transition in liquid sulfur with a differential scanning calorimeter. J of Polymer Science: Part B: Polymer Physics 1974, 12: 815–818. 10.1002/pol.1974.180120415View Article
- Wang H, Yang Y: Graphene-wrapped sulfur particles as a rechargeable lithium-sulfur battery cathode material with high capacity and cycling stability. Nano Lett 2011, 11: 644–2647.
- Hummers WS, Ofeman RE: Preparation of graphitic oxide. J Am Chem Soc 1958, 80(6):1339. 10.1021/ja01539a017View Article
- Currell BR, Williams AJ: Thermal analysis of elemental sulphur. Thermochimica Acta 1974, 9: 255–259. 10.1016/0040-6031(74)80005-5View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.